#------------------------------------------------------------------------------
#$Date: 2021-11-23 10:34:50 +0200 (Tue, 23 Nov 2021) $
#$Revision: 270822 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/32/90/4329003.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4329003
loop_
_publ_author_name
'Zheng-Guo Lin'
'Bo Wang'
'Jie Cao'
'Bao-Kuan Chen'
'Yuan-Zhe Gao'
'Ying-Nan Chi'
'Chong Xu'
'Xian-Qiang Huang'
'Ruo-Dan Han'
'Shuang-Yue Su'
'Chang-Wen Hu'
_publ_contact_author_email       cwhu@bit.edu.cn
_publ_contact_author_name        'Changwen Hu'
_publ_section_title
;
 Cation-Induced Synthesis of New Polyoxopalladates
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4435
_journal_page_last               4437
_journal_paper_doi               10.1021/ic300428g
_journal_volume                  51
_journal_year                    2012
_chemical_formula_sum            'K5 O61 Pd15 Se10'
_chemical_formula_weight         3557.10
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            12
_cell_length_a                   34.428(2)
_cell_length_b                   24.9433(17)
_cell_length_c                   23.3876(16)
_cell_measurement_reflns_used    9954
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.32
_cell_measurement_theta_min      2.39
_cell_volume                     20084(2)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.981
_diffrn_measured_fraction_theta_max 0.981
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0754
_diffrn_reflns_av_sigmaI/netI    0.0755
_diffrn_reflns_limit_h_max       43
_diffrn_reflns_limit_h_min       -41
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -33
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            61300
_diffrn_reflns_theta_full        28.36
_diffrn_reflns_theta_max         28.36
_diffrn_reflns_theta_min         1.01
_exptl_absorpt_coefficient_mu    9.783
_exptl_absorpt_correction_T_max  0.209
_exptl_absorpt_correction_T_min  0.066
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker SMART'
_exptl_crystal_colour            Redbrown
_exptl_crystal_density_diffrn    3.529
_exptl_crystal_description       Block
_exptl_crystal_F_000             19356
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.16
_refine_diff_density_max         3.545
_refine_diff_density_min         -3.332
_refine_diff_density_rms         0.430
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     663
_refine_ls_number_reflns         12829
_refine_ls_number_restraints     852
_refine_ls_restrained_S_all      1.094
_refine_ls_R_factor_all          0.1086
_refine_ls_R_factor_gt           0.0653
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1361P)²+83.9947P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1922
_refine_ls_wR_factor_ref         0.2319
_reflns_number_gt                8094
_reflns_number_total             13075
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic300428g_si_002_3.cif
_cod_data_source_block           compound2
_cod_depositor_comments
;

2021-11-23
Z value and formula fixed to values more according to usual
chemical conventions.                 miguel
;
_cod_original_formula_sum            'K30 O366 Pd90 Se60'
_cod_original_formula_weight         21342.60
_cod_original_formula_units_Z            2
_cod_database_code               4329003
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'x, -y, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'x+1/2, -y+1/2, z-1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
K1 K 0.0000 0.8957(3) 0.6289(3) 0.0828(19) Uani 1 2 d SU
K2 K 0.16223(10) 0.94160(18) 0.2500 0.0485(12) Uani 1 2 d SU
K3 K 0.0000 0.4309(3) 0.2500 0.063(2) Uani 1 4 d SU
K4 K 0.16782(14) 0.6188(4) 0.3487(4) 0.140(2) Uani 1 1 d U
K5 K 0.16542(7) 0.79138(16) 0.43565(14) 0.0487(9) Uani 1 1 d U
K6 K 0.0000 0.6813(2) 0.56503(19) 0.0533(12) Uani 1 2 d SU
O1 O 0.0000 0.7423(7) 0.2500 0.030(3) Uani 1 4 d SU
O2 O 0.1671(3) 0.7494(5) 0.7500 0.033(2) Uani 1 2 d SU
O3 O 0.12925(19) 0.6713(3) 0.6914(3) 0.0255(16) Uani 1 1 d U
O4 O 0.2120(3) 0.5805(4) 0.6165(4) 0.049(2) Uani 1 1 d U
O5 O 0.2670(2) 0.6543(4) 0.6007(4) 0.042(2) Uani 1 1 d U
O6 O 0.20976(19) 0.6750(3) 0.6916(3) 0.0254(16) Uani 1 1 d U
O7 O 0.2064(2) 0.7807(3) 0.6565(3) 0.0271(16) Uani 1 1 d U
O8 O 0.2618(2) 0.7554(4) 0.5643(4) 0.040(2) Uani 1 1 d U
O9 O 0.2620(2) 0.8571(4) 0.6008(4) 0.039(2) Uani 1 1 d U
O10 O 0.2026(2) 0.8198(4) 0.5375(3) 0.0395(19) Uani 1 1 d U
O11 O 0.2610(3) 0.9189(4) 0.6930(4) 0.050(2) Uani 1 1 d U
O12 O 0.2015(3) 0.9633(5) 0.7500 0.040(3) Uani 1 2 d SU
O13 O 0.1243(3) 0.9607(5) 0.7500 0.042(3) Uani 1 2 d SU
O14 O 0.0665(3) 0.9112(4) 0.6928(5) 0.053(2) Uani 1 1 d U
O15 O 0.1251(3) 0.8436(4) 0.7500 0.025(2) Uani 1 2 d SU
O16 O 0.0662(3) 0.8474(5) 0.6018(4) 0.056(2) Uani 1 1 d U
O17 O 0.0677(2) 0.7455(4) 0.5692(4) 0.045(2) Uani 1 1 d U
O18 O 0.1247(2) 0.7763(3) 0.6567(3) 0.0277(16) Uani 1 1 d U
O19 O 0.1251(2) 0.8123(4) 0.5378(4) 0.044(2) Uani 1 1 d U
O20 O 0.2690(2) 0.5886(4) 0.6924(4) 0.043(2) Uani 1 1 d U
O21 O 0.0392(3) 0.5282(5) 0.2500 0.050(3) Uani 1 2 d SU
O22 O 0.0405(3) 0.6454(4) 0.2500 0.022(2) Uani 1 2 d SU
O23 O 0.0974(3) 0.5740(4) 0.3069(5) 0.056(2) Uani 1 1 d U
O24 O 0.0987(3) 0.6371(4) 0.3984(4) 0.052(2) Uani 1 1 d U
O25 O 0.0954(2) 0.7383(4) 0.4351(4) 0.044(2) Uani 1 1 d U
O26 O 0.0405(2) 0.7104(3) 0.3445(3) 0.0277(16) Uani 1 1 d U
O27 O 0.0407(2) 0.8155(3) 0.3088(3) 0.0301(17) Uani 1 1 d U
O28 O 0.0957(3) 0.9076(4) 0.3078(4) 0.053(2) Uani 1 1 d U
O29 O 0.0385(2) 0.6694(4) 0.4622(4) 0.047(2) Uani 1 1 d U
O30 O 0.0986(3) 0.8398(4) 0.3980(4) 0.048(2) Uani 1 1 d U
O31 O 0.0395(3) 0.9087(4) 0.3858(5) 0.057(3) Uani 1 1 d U
O32 O 0.2052(3) 0.8461(4) 0.7500 0.027(2) Uani 1 2 d SU
O33 O 0.1328(3) 0.5757(4) 0.6162(4) 0.050(2) Uani 1 1 d U
O34 O 0.0734(2) 0.6430(4) 0.5988(4) 0.043(2) Uani 1 1 d U
O35 O 0.1625(4) 1.0011(10) 0.1330(9) 0.137(7) Uani 1 1 d U
O36 O 0.0000 0.3189(11) 0.2990(11) 0.148(7) Uani 1 2 d SU
O37 O 0.0000 0.5004(12) 0.3667(13) 0.151(8) Uani 1 2 d SU
O38 O 0.0000 0.5702(8) 0.5276(11) 0.124(7) Uani 1 2 d SU
O39 O 0.1687(4) 0.6824(8) 0.5159(8) 0.132(6) Uani 1 1 d U
O40 O 0.1612(4) 0.9149(7) 0.4867(8) 0.114(5) Uani 1 1 d U
O41 O 0.1664(3) 0.7258(9) 0.3377(8) 0.108(4) Uani 1 1 d U
O42 O 0.1703(4) 0.5347(8) 0.3659(9) 0.135(4) Uani 1 1 d U
O43 O 0.0000 0.9970(8) 0.6335(13) 0.145(8) Uani 1 2 d SU
O44 O 0.0000 0.9047(11) 0.4993(10) 0.135(7) Uani 1 2 d SU
O45 O 0.1729(4) 0.4337(7) 0.4988(7) 0.110(5) Uani 1 1 d U
O46 O 0.0915(6) 0.9580(8) 0.9437(13) 0.206(11) Uani 1 1 d .
O47 O 0.1667(7) 0.221(3) 0.7500 0.42(5) Uani 1 2 d S
O48 O 0.2490(7) 0.5354(9) 0.4391(11) 0.184(7) Uani 1 1 d U
O49 O 0.1677(5) 0.6822(13) 0.2500 0.119(6) Uani 1 2 d SU
O50 O 0.3009(10) 0.5000 0.5000 0.237(10) Uani 1 2 d SU
O51 O 0.0000 0.7674(10) 0.6616(9) 0.104(4) Uani 1 2 d SU
O52 O 0.0000 0.8454(9) 0.7228(9) 0.140(5) Uani 1 2 d SU
O53 O 0.1724(2) 0.4936(3) 0.4293(4) 0.0337(19) Uani 1 1 d U
O54 O 0.0807(5) 0.5350(8) 0.4555(8) 0.137(4) Uani 1 1 d U
O55 O 0.0742(2) 0.5798(4) 0.6920(4) 0.039(2) Uani 1 1 d U
Pd1 Pd 0.0000 0.69079(5) 0.40205(5) 0.0253(3) Uani 1 2 d S
Pd2 Pd 0.16483(2) 0.79725(4) 0.59891(4) 0.0239(2) Uani 1 1 d .
Pd3 Pd 0.06869(2) 0.77581(4) 0.37004(4) 0.0268(2) Uani 1 1 d .
Pd4 Pd 0.23620(2) 0.71666(4) 0.62995(3) 0.0247(2) Uani 1 1 d .
Pd5 Pd 0.09897(2) 0.70947(4) 0.63022(4) 0.0260(2) Uani 1 1 d .
Pd6 Pd 0.09579(2) 0.84348(4) 0.67608(4) 0.0272(2) Uani 1 1 d .
Pd7 Pd 0.23346(2) 0.84962(4) 0.67577(4) 0.0252(2) Uani 1 1 d .
Pd8 Pd 0.06909(2) 0.64299(4) 0.32427(4) 0.0259(2) Uani 1 1 d .
Pd9 Pd 0.16390(3) 0.90149(5) 0.7500 0.0248(3) Uani 1 2 d S
Pd10 Pd 0.0000 0.58913(7) 0.2500 0.0248(4) Uani 1 4 d S
Pd11 Pd 0.06816(3) 0.86042(6) 0.2500 0.0302(3) Uani 1 2 d S
Pd12 Pd 0.23933(3) 0.63265(5) 0.7500 0.0250(3) Uani 1 2 d S
Pd13 Pd 0.10177(3) 0.62657(5) 0.7500 0.0253(3) Uani 1 2 d S
Pd14 Pd 0.0000 0.86104(5) 0.34647(6) 0.0312(3) Uani 1 2 d S
Pd15 Pd 0.17072(2) 0.62657(4) 0.65469(4) 0.0284(2) Uani 1 1 d .
Se1 Se 0.25068(5) 0.95899(7) 0.7500 0.0300(4) Uani 1 2 d S
Se2 Se 0.08796(4) 0.53431(7) 0.2500 0.0287(4) Uani 1 2 d S
Se3 Se 0.07515(5) 0.95207(7) 0.7500 0.0336(4) Uani 1 2 d S
Se4 Se 0.08734(3) 0.67559(5) 0.45792(5) 0.0306(3) Uani 1 1 d .
Se5 Se 0.25159(3) 0.81774(5) 0.54188(5) 0.0289(3) Uani 1 1 d .
Se6 Se 0.07671(3) 0.80803(5) 0.54327(5) 0.0311(3) Uani 1 1 d .
Se7 Se 0.08864(4) 0.90388(6) 0.37875(6) 0.0383(3) Uani 1 1 d .
Se8 Se 0.26042(4) 0.58964(5) 0.62142(5) 0.0337(3) Uani 1 1 d .
Se9 Se 0.08338(4) 0.57997(6) 0.62149(6) 0.0354(3) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pd Pd -0.9988 1.0072 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O43 K1 O52 117.2(9) . .
O43 K1 O16 117.6(3) . 12
O52 K1 O16 89.0(4) . 12
O43 K1 O16 117.6(3) . .
O52 K1 O16 89.0(4) . .
O16 K1 O16 118.3(5) 12 .
O43 K1 O14 80.6(4) . .
O52 K1 O14 66.4(4) . .
O16 K1 O14 154.7(5) 12 .
O16 K1 O14 58.7(3) . .
O43 K1 O14 80.6(4) . 12
O52 K1 O14 66.4(4) . 12
O16 K1 O14 58.7(3) 12 12
O16 K1 O14 154.7(5) . 12
O14 K1 O14 112.1(5) . 12
O43 K1 O44 88.3(9) . .
O52 K1 O44 154.5(8) . .
O16 K1 O44 78.2(4) 12 .
O16 K1 O44 78.2(4) . .
O14 K1 O44 122.0(3) . .
O14 K1 O44 122.0(3) 12 .
O43 K1 O51 164.1(8) . .
O52 K1 O51 46.8(6) . .
O16 K1 O51 67.3(3) 12 .
O16 K1 O51 67.3(3) . .
O14 K1 O51 90.6(4) . .
O14 K1 O51 90.6(4) 12 .
O44 K1 O51 107.7(6) . .
O43 K1 Pd6 109.7(3) . 12
O52 K1 Pd6 64.39(14) . 12
O16 K1 Pd6 31.7(2) 12 12
O16 K1 Pd6 132.4(4) . 12
O14 K1 Pd6 128.7(3) . 12
O14 K1 Pd6 32.0(2) 12 12
O44 K1 Pd6 108.8(2) . 12
O51 K1 Pd6 65.77(14) . 12
O43 K1 Pd6 109.7(3) . .
O52 K1 Pd6 64.39(14) . .
O16 K1 Pd6 132.4(4) 12 .
O16 K1 Pd6 31.7(2) . .
O14 K1 Pd6 32.0(2) . .
O14 K1 Pd6 128.7(3) 12 .
O44 K1 Pd6 108.8(2) . .
O51 K1 Pd6 65.77(14) . .
Pd6 K1 Pd6 125.2(2) 12 .
O12 K2 O13 57.8(4) 11_575 11_575
O12 K2 O28 132.1(3) 11_575 10_556
O13 K2 O28 83.2(3) 11_575 10_556
O12 K2 O28 132.1(3) 11_575 .
O13 K2 O28 83.2(3) 11_575 .
O28 K2 O28 57.9(4) 10_556 .
O12 K2 O20 79.4(3) 11_575 13_566
O13 K2 O20 129.1(3) 11_575 13_566
O28 K2 O20 146.8(4) 10_556 13_566
O28 K2 O20 112.1(3) . 13_566
O12 K2 O20 79.4(3) 11_575 6_564
O13 K2 O20 129.1(3) 11_575 6_564
O28 K2 O20 112.1(3) 10_556 6_564
O28 K2 O20 146.8(4) . 6_564
O20 K2 O20 56.9(3) 13_566 6_564
O12 K2 O35 65.4(4) 11_575 10_556
O13 K2 O35 65.3(4) 11_575 10_556
O28 K2 O35 125.0(4) 10_556 10_556
O28 K2 O35 73.9(4) . 10_556
O20 K2 O35 72.9(4) 13_566 10_556
O20 K2 O35 122.9(4) 6_564 10_556
O12 K2 O35 65.4(4) 11_575 .
O13 K2 O35 65.3(4) 11_575 .
O28 K2 O35 73.9(4) 10_556 .
O28 K2 O35 125.0(4) . .
O20 K2 O35 122.9(4) 13_566 .
O20 K2 O35 72.9(4) 6_564 .
O35 K2 O35 123.1(9) 10_556 .
O12 K2 Pd11 151.7(3) 11_575 .
O13 K2 Pd11 93.8(3) 11_575 .
O28 K2 Pd11 31.0(2) 10_556 .
O28 K2 Pd11 31.0(2) . .
O20 K2 Pd11 124.7(2) 13_566 .
O20 K2 Pd11 124.7(2) 6_564 .
O35 K2 Pd11 104.8(3) 10_556 .
O35 K2 Pd11 104.8(3) . .
O12 K2 Pd12 89.0(3) 11_575 13_566
O13 K2 Pd12 146.8(3) 11_575 13_566
O28 K2 Pd12 125.0(3) 10_556 13_566
O28 K2 Pd12 125.0(3) . 13_566
O20 K2 Pd12 30.34(18) 13_566 13_566
O20 K2 Pd12 30.34(18) 6_564 13_566
O35 K2 Pd12 103.0(3) 10_556 13_566
O35 K2 Pd12 103.0(3) . 13_566
Pd11 K2 Pd12 119.33(12) . 13_566
O12 K2 Pd9 28.8(2) 11_575 11_575
O13 K2 Pd9 29.0(3) 11_575 11_575
O28 K2 Pd9 108.4(3) 10_556 11_575
O28 K2 Pd9 108.4(3) . 11_575
O20 K2 Pd9 104.7(2) 13_566 11_575
O20 K2 Pd9 104.7(2) 6_564 11_575
O35 K2 Pd9 61.5(4) 10_556 11_575
O35 K2 Pd9 61.5(4) . 11_575
Pd11 K2 Pd9 122.85(11) . 11_575
Pd12 K2 Pd9 117.82(10) 13_566 11_575
O12 K2 Se1 21.2(2) 11_575 11_575
O13 K2 Se1 79.0(3) 11_575 11_575
O28 K2 Se1 145.9(2) 10_556 11_575
O28 K2 Se1 145.9(2) . 11_575
O20 K2 Se1 61.2(2) 13_566 11_575
O20 K2 Se1 61.2(2) 6_564 11_575
O35 K2 Se1 72.3(3) 10_556 11_575
O35 K2 Se1 72.3(3) . 11_575
Pd11 K2 Se1 172.86(13) . 11_575
Pd12 K2 Se1 67.81(7) 13_566 11_575
Pd9 K2 Se1 50.00(6) 11_575 11_575
O21 K3 O21 58.2(5) . 3
O21 K3 O55 120.5(3) . 2_564
O21 K3 O55 69.7(3) 3 2_564
O21 K3 O55 69.7(3) . 4_566
O21 K3 O55 120.5(3) 3 4_566
O55 K3 O55 169.4(5) 2_564 4_566
O21 K3 O55 120.5(3) . 9_566
O21 K3 O55 69.7(3) 3 9_566
O55 K3 O55 55.6(3) 2_564 9_566
O55 K3 O55 123.2(3) 4_566 9_566
O21 K3 O55 69.7(3) . 11_565
O21 K3 O55 120.5(3) 3 11_565
O55 K3 O55 123.2(3) 2_564 11_565
O55 K3 O55 55.6(3) 4_566 11_565
O55 K3 O55 169.4(5) 9_566 11_565
O21 K3 O36 144.0(3) . 10_556
O21 K3 O36 144.0(3) 3 10_556
O55 K3 O36 74.8(3) 2_564 10_556
O55 K3 O36 95.3(3) 4_566 10_556
O55 K3 O36 95.3(3) 9_566 10_556
O55 K3 O36 74.8(3) 11_565 10_556
O21 K3 O36 144.0(3) . .
O21 K3 O36 144.0(3) 3 .
O55 K3 O36 95.3(3) 2_564 .
O55 K3 O36 74.8(3) 4_566 .
O55 K3 O36 74.8(3) 9_566 .
O55 K3 O36 95.3(3) 11_565 .
O36 K3 O36 44.6(10) 10_556 .
O21 K3 O37 62.1(5) . .
O21 K3 O37 62.1(5) 3 .
O55 K3 O37 116.3(2) 2_564 .
O55 K3 O37 69.9(3) 4_566 .
O55 K3 O37 69.9(3) 9_566 .
O55 K3 O37 116.3(2) 11_565 .
O36 K3 O37 144.7(7) 10_556 .
O36 K3 O37 100.1(7) . .
O21 K3 O37 62.1(5) . 10_556
O21 K3 O37 62.1(5) 3 10_556
O55 K3 O37 69.9(3) 2_564 10_556
O55 K3 O37 116.3(2) 4_566 10_556
O55 K3 O37 116.3(2) 9_566 10_556
O55 K3 O37 69.9(3) 11_565 10_556
O36 K3 O37 100.1(7) 10_556 10_556
O36 K3 O37 144.7(7) . 10_556
O37 K3 O37 115.1(11) . 10_556
O21 K3 Pd13 83.2(2) . 11_565
O21 K3 Pd13 141.3(3) 3 11_565
O55 K3 Pd13 141.2(2) 2_564 11_565
O55 K3 Pd13 31.90(17) 4_566 11_565
O55 K3 Pd13 141.2(2) 9_566 11_565
O55 K3 Pd13 31.90(17) 11_565 11_565
O36 K3 Pd13 69.48(13) 10_556 11_565
O36 K3 Pd13 69.48(13) . 11_565
O37 K3 Pd13 101.72(17) . 11_565
O37 K3 Pd13 101.72(17) 10_556 11_565
O21 K3 Pd13 141.3(3) . 9_566
O21 K3 Pd13 83.2(2) 3 9_566
O55 K3 Pd13 31.90(17) 2_564 9_566
O55 K3 Pd13 141.2(2) 4_566 9_566
O55 K3 Pd13 31.90(17) 9_566 9_566
O55 K3 Pd13 141.2(2) 11_565 9_566
O36 K3 Pd13 69.48(13) 10_556 9_566
O36 K3 Pd13 69.48(13) . 9_566
O37 K3 Pd13 101.72(17) . 9_566
O37 K3 Pd13 101.72(17) 10_556 9_566
Pd13 K3 Pd13 135.49(19) 11_565 9_566
O42 K4 O41 174.5(8) . .
O42 K4 O24 96.9(6) . .
O41 K4 O24 81.7(4) . .
O42 K4 O9 95.7(5) . 13_566
O41 K4 O9 80.8(4) . 13_566
O24 K4 O9 123.6(4) . 13_566
O42 K4 O49 135.2(9) . .
O41 K4 O49 50.1(7) . .
O24 K4 O49 105.0(5) . .
O9 K4 O49 103.4(5) 13_566 .
O42 K4 O11 72.6(5) . 13_566
O41 K4 O11 108.5(4) . 13_566
O24 K4 O11 169.3(5) . 13_566
O9 K4 O11 57.0(3) 13_566 13_566
O49 K4 O11 84.5(5) . 13_566
O42 K4 O23 73.3(5) . .
O41 K4 O23 110.0(4) . .
O24 K4 O23 57.3(3) . .
O9 K4 O23 168.7(5) 13_566 .
O49 K4 O23 86.4(5) . .
O11 K4 O23 119.6(4) 13_566 .
O42 K4 Pd8 103.8(4) . .
O41 K4 Pd8 78.2(3) . .
O24 K4 Pd8 35.0(2) . .
O9 K4 Pd8 152.1(4) 13_566 .
O49 K4 Pd8 76.5(4) . .
O11 K4 Pd8 148.3(4) 13_566 .
O23 K4 Pd8 35.2(2) . .
O42 K4 Pd7 102.2(4) . 13_566
O41 K4 Pd7 77.3(3) . 13_566
O24 K4 Pd7 152.1(4) . 13_566
O9 K4 Pd7 34.72(19) 13_566 13_566
O49 K4 Pd7 75.1(4) . 13_566
O11 K4 Pd7 34.6(2) 13_566 13_566
O23 K4 Pd7 148.4(4) . 13_566
Pd8 K4 Pd7 150.4(3) . 13_566
O42 K4 K4 100.8(6) . 10_556
O41 K4 K4 84.5(4) . 10_556
O24 K4 K4 115.6(3) . 10_556
O9 K4 K4 115.4(2) 13_566 10_556
O49 K4 K4 34.4(6) . 10_556
O11 K4 K4 69.6(3) 13_566 10_556
O23 K4 K4 69.9(3) . 10_556
Pd8 K4 K4 80.61(14) . 10_556
Pd7 K4 K4 80.69(14) 13_566 10_556
O42 K4 K5 143.9(7) . .
O41 K4 K5 30.8(4) . .
O24 K4 K5 69.3(3) . .
O9 K4 K5 68.6(3) 13_566 .
O49 K4 K5 80.9(6) . .
O11 K4 K5 117.9(3) 13_566 .
O23 K4 K5 119.2(3) . .
Pd8 K4 K5 84.09(15) . .
Pd7 K4 K5 83.36(16) 13_566 .
K4 K4 K5 115.29(12) 10_556 .
O30 K5 O25 58.4(3) . .
O30 K5 O8 161.1(3) . 13_566
O25 K5 O8 126.2(4) . 13_566
O30 K5 O10 123.1(3) . .
O25 K5 O10 121.9(3) . .
O8 K5 O10 72.0(3) 13_566 .
O30 K5 O19 77.1(3) . .
O25 K5 O19 70.2(3) . .
O8 K5 O19 121.7(3) 13_566 .
O10 K5 O19 57.0(3) . .
O30 K5 O41 90.3(4) . .
O25 K5 O41 74.1(3) . .
O8 K5 O41 75.2(3) 13_566 .
O10 K5 O41 146.6(4) . .
O19 K5 O41 143.6(4) . .
O30 K5 O5 112.5(3) . 13_566
O25 K5 O5 162.2(3) . 13_566
O8 K5 O5 57.0(3) 13_566 13_566
O10 K5 O5 75.9(3) . 13_566
O19 K5 O5 125.0(3) . 13_566
O41 K5 O5 91.4(4) . 13_566
O30 K5 O39 124.9(3) . .
O25 K5 O39 68.7(3) . .
O8 K5 O39 67.8(3) 13_566 .
O10 K5 O39 73.1(4) . .
O19 K5 O39 71.8(4) . .
O41 K5 O39 89.1(6) . .
O5 K5 O39 122.5(3) 13_566 .
O30 K5 O40 70.6(3) . .
O25 K5 O40 114.3(3) . .
O8 K5 O40 115.7(3) 13_566 .
O10 K5 O40 58.5(4) . .
O19 K5 O40 59.9(4) . .
O41 K5 O40 146.7(6) . .
O5 K5 O40 72.4(3) 13_566 .
O39 K5 O40 124.2(5) . .
O30 K5 Pd3 32.4(2) . .
O25 K5 Pd3 32.4(2) . .
O8 K5 Pd3 140.7(2) 13_566 .
O10 K5 Pd3 142.67(19) . .
O19 K5 Pd3 85.81(18) . .
O41 K5 Pd3 67.1(2) . .
O5 K5 Pd3 132.0(2) 13_566 .
O39 K5 Pd3 100.4(3) . .
O40 K5 Pd3 102.0(3) . .
O30 K5 Pd4 130.9(2) . 13_566
O25 K5 Pd4 140.3(2) . 13_566
O8 K5 Pd4 32.10(18) 13_566 13_566
O10 K5 Pd4 87.01(18) . 13_566
O19 K5 Pd4 144.02(19) . 13_566
O41 K5 Pd4 67.8(2) . 13_566
O5 K5 Pd4 32.04(18) 13_566 13_566
O39 K5 Pd4 99.1(3) . 13_566
O40 K5 Pd4 103.8(3) . 13_566
Pd3 K5 Pd4 130.12(9) . 13_566
O30 K5 Pd2 107.4(2) . .
O25 K5 Pd2 91.1(2) . .
O8 K5 Pd2 91.2(2) 13_566 .
O10 K5 Pd2 30.84(17) . .
O19 K5 Pd2 30.85(17) . .
O41 K5 Pd2 146.7(5) . .
O5 K5 Pd2 106.7(2) 13_566 .
O39 K5 Pd2 57.6(3) . .
O40 K5 Pd2 66.6(3) . .
Pd3 K5 Pd2 114.52(7) . .
Pd4 K5 Pd2 114.74(7) 13_566 .
O29 K6 O29 57.4(4) 12 .
O29 K6 O34 77.1(3) 12 12
O29 K6 O34 129.7(3) . 12
O29 K6 O34 129.7(3) 12 .
O29 K6 O34 77.1(3) . .
O34 K6 O34 127.8(4) 12 .
O29 K6 O17 119.1(3) 12 .
O29 K6 O17 72.2(3) . .
O34 K6 O17 157.2(3) 12 .
O34 K6 O17 56.1(3) . .
O29 K6 O17 72.2(3) 12 12
O29 K6 O17 119.1(3) . 12
O34 K6 O17 56.1(3) 12 12
O34 K6 O17 157.2(3) . 12
O17 K6 O17 110.9(4) . 12
O29 K6 O38 68.6(5) 12 .
O29 K6 O38 68.6(5) . .
O34 K6 O38 76.2(3) 12 .
O34 K6 O38 76.2(3) . .
O17 K6 O38 123.4(2) . .
O17 K6 O38 123.4(2) 12 .
O29 K6 O51 134.8(4) 12 .
O29 K6 O51 134.8(4) . .
O34 K6 O51 91.7(3) 12 .
O34 K6 O51 91.7(3) . .
O17 K6 O51 65.5(3) . .
O17 K6 O51 65.5(3) 12 .
O38 K6 O51 151.1(7) . .
O29 K6 O36 150.5(2) 12 9_566
O29 K6 O36 150.5(2) . 9_566
O34 K6 O36 73.7(3) 12 9_566
O34 K6 O36 73.7(3) . 9_566
O17 K6 O36 88.1(3) . 9_566
O17 K6 O36 88.1(3) 12 9_566
O38 K6 O36 107.5(7) . 9_566
O51 K6 O36 43.6(6) . 9_566
O29 K6 Pd5 143.1(2) 12 .
O29 K6 Pd5 86.48(18) . .
O34 K6 Pd5 139.1(2) 12 .
O34 K6 Pd5 31.2(2) . .
O17 K6 Pd5 30.97(18) . .
O17 K6 Pd5 128.3(3) 12 .
O38 K6 Pd5 107.3(2) . .
O51 K6 Pd5 65.26(10) . .
O36 K6 Pd5 66.35(12) 9_566 .
O29 K6 Pd5 86.48(18) 12 12
O29 K6 Pd5 143.1(2) . 12
O34 K6 Pd5 31.2(2) 12 12
O34 K6 Pd5 139.1(2) . 12
O17 K6 Pd5 128.3(3) . 12
O17 K6 Pd5 30.97(18) 12 12
O38 K6 Pd5 107.3(2) . 12
O51 K6 Pd5 65.26(10) . 12
O36 K6 Pd5 66.35(12) 9_566 12
Pd5 K6 Pd5 127.53(13) . 12
O29 K6 Pd1 30.41(18) 12 .
O29 K6 Pd1 30.41(18) . .
O34 K6 Pd1 107.5(2) 12 .
O34 K6 Pd1 107.5(2) . .
O17 K6 Pd1 89.9(2) . .
O17 K6 Pd1 89.9(2) 12 .
O38 K6 Pd1 76.0(5) . .
O51 K6 Pd1 132.9(5) . .
O36 K6 Pd1 176.5(5) 9_566 .
Pd5 K6 Pd1 112.90(7) . .
Pd5 K6 Pd1 112.90(7) 12 .
Pd15 O3 Pd13 108.6(3) . .
Pd15 O3 Pd5 109.2(3) . .
Pd13 O3 Pd5 120.4(3) . .
Se8 O4 Pd15 125.8(5) . .
Se8 O5 Pd4 124.7(4) . .
Se8 O5 K5 130.6(4) . 13_566
Pd4 O5 K5 99.6(4) . 13_566
Pd4 O6 Pd15 108.0(3) . .
Pd4 O6 Pd12 122.3(3) . .
Pd15 O6 Pd12 108.5(3) . .
Pd4 O7 Pd7 121.1(3) . .
Pd4 O7 Pd2 108.8(3) . .
Pd7 O7 Pd2 107.8(4) . .
Se5 O8 Pd4 126.2(5) . .
Se5 O8 K5 125.5(4) . 13_566
Pd4 O8 K5 101.2(3) . 13_566
Se5 O9 Pd7 122.6(4) . .
Se5 O9 K4 130.4(4) . 13_566
Pd7 O9 K4 94.3(4) . 13_566
Se5 O10 Pd2 126.3(4) . .
Se5 O10 K5 120.1(4) . .
Pd2 O10 K5 103.9(3) . .
Se1 O11 Pd7 124.3(5) . .
Se1 O11 K4 130.7(5) . 13_566
Pd7 O11 K4 93.1(4) . 13_566
Se1 O12 Pd9 126.4(6) . .
Se1 O12 K2 123.3(6) . 11_576
Pd9 O12 K2 110.3(5) . 11_576
Se3 O13 Pd9 125.4(7) . .
Se3 O13 K2 125.5(6) . 11_576
Pd9 O13 K2 109.2(5) . 11_576
Se3 O14 Pd6 124.6(5) . .
Se3 O14 K1 130.6(5) . .
Pd6 O14 K1 101.2(4) . .
Pd9 O15 Pd6 110.1(3) . .
Pd9 O15 Pd6 110.1(3) . 10_557
Pd6 O15 Pd6 119.5(5) . 10_557
Se6 O16 Pd6 123.4(5) . .
Se6 O16 K1 128.9(5) . .
Pd6 O16 K1 104.5(4) . .
Se6 O17 Pd5 124.6(5) . .
Se6 O17 K6 131.0(4) . .
Pd5 O17 K6 102.3(4) . .
Pd5 O18 Pd2 108.5(3) . .
Pd5 O18 Pd6 123.4(4) . .
Pd2 O18 Pd6 106.1(4) . .
Se6 O19 Pd2 127.5(5) . .
Se6 O19 K5 123.0(4) . .
Pd2 O19 K5 103.5(3) . .
Se8 O20 Pd12 124.2(4) . .
Se8 O20 K2 128.2(4) . 13_566
Pd12 O20 K2 104.5(4) . 13_566
Se2 O21 Pd10 126.4(7) . .
Se2 O21 K3 124.3(6) . .
Pd10 O21 K3 109.3(5) . .
Pd10 O22 Pd8 109.0(3) . .
Pd10 O22 Pd8 109.0(3) . 10_556
Pd8 O22 Pd8 120.8(4) . 10_556
Se2 O23 Pd8 124.3(5) . .
Se2 O23 K4 131.7(5) . .
Pd8 O23 K4 90.4(4) . .
Se4 O24 Pd8 122.4(5) . .
Se4 O24 K4 129.8(5) . .
Pd8 O24 K4 95.0(4) . .
Se4 O25 Pd3 126.9(5) . .
Se4 O25 K5 126.4(4) . .
Pd3 O25 K5 100.4(4) . .
Pd3 O26 Pd1 109.8(4) . .
Pd3 O26 Pd8 121.2(4) . .
Pd1 O26 Pd8 107.2(4) . .
Pd3 O27 Pd14 107.7(3) . .
Pd3 O27 Pd11 122.8(3) . .
Pd14 O27 Pd11 108.2(4) . .
Se7 O28 Pd11 123.9(5) . .
Se7 O28 K2 127.9(4) . .
Pd11 O28 K2 103.8(4) . .
Se4 O29 Pd1 126.3(5) . .
Se4 O29 K6 121.2(4) . .
Pd1 O29 K6 105.3(3) . .
Se7 O30 Pd3 123.9(5) . .
Se7 O30 K5 132.1(4) . .
Pd3 O30 K5 100.7(4) . .
Se7 O31 Pd14 125.5(5) . .
Pd9 O32 Pd7 108.6(3) . 10_557
Pd9 O32 Pd7 108.6(3) . .
Pd7 O32 Pd7 121.3(5) 10_557 .
Se9 O33 Pd15 124.7(5) . .
Se9 O34 Pd5 124.1(4) . .
Se9 O34 K6 125.8(4) . .
Pd5 O34 K6 102.5(4) . .
K3 O36 K6 112.3(8) . 9_566
K4 O41 K5 120.0(8) . .
O53 O42 K4 135.6(12) . .
K4 O49 K4 111.2(12) 10_556 .
K6 O51 K1 120.1(7) . .
O52 O52 K1 150.3(5) 10_557 .
Se9 O55 Pd13 124.7(5) . .
Se9 O55 K3 128.6(4) . 9_566
Pd13 O55 K3 98.8(3) . 9_566
O26 Pd1 O26 88.4(4) 12 .
O26 Pd1 O29 177.2(3) 12 .
O26 Pd1 O29 94.4(3) . .
O26 Pd1 O29 94.4(3) 12 12
O26 Pd1 O29 177.2(3) . 12
O29 Pd1 O29 82.9(5) . 12
O26 Pd1 Pd8 36.5(2) 12 12
O26 Pd1 Pd8 103.0(2) . 12
O29 Pd1 Pd8 141.8(3) . 12
O29 Pd1 Pd8 79.0(3) 12 12
O26 Pd1 Pd8 103.0(2) 12 .
O26 Pd1 Pd8 36.5(2) . .
O29 Pd1 Pd8 79.0(3) . .
O29 Pd1 Pd8 141.8(3) 12 .
Pd8 Pd1 Pd8 95.12(4) 12 .
O26 Pd1 K6 133.5(2) 12 .
O26 Pd1 K6 133.5(2) . .
O29 Pd1 K6 44.2(3) . .
O29 Pd1 K6 44.2(3) 12 .
Pd8 Pd1 K6 122.70(5) 12 .
Pd8 Pd1 K6 122.70(5) . .
O18 Pd2 O7 89.2(3) . .
O18 Pd2 O19 93.4(3) . .
O7 Pd2 O19 176.8(3) . .
O18 Pd2 O10 176.5(3) . .
O7 Pd2 O10 94.3(3) . .
O19 Pd2 O10 83.1(4) . .
O18 Pd2 Pd6 37.0(2) . .
O7 Pd2 Pd6 103.0(2) . .
O19 Pd2 Pd6 80.1(3) . .
O10 Pd2 Pd6 141.3(3) . .
O18 Pd2 Pd5 35.6(2) . .
O7 Pd2 Pd5 102.1(2) . .
O19 Pd2 Pd5 79.1(3) . .
O10 Pd2 Pd5 143.3(3) . .
Pd6 Pd2 Pd5 66.15(3) . .
O18 Pd2 Pd7 103.5(2) . .
O7 Pd2 Pd7 36.1(2) . .
O19 Pd2 Pd7 144.4(3) . .
O10 Pd2 Pd7 79.2(2) . .
Pd6 Pd2 Pd7 94.79(3) . .
Pd5 Pd2 Pd7 131.11(4) . .
O18 Pd2 Pd4 102.0(2) . .
O7 Pd2 Pd4 35.5(2) . .
O19 Pd2 Pd4 141.8(3) . .
O10 Pd2 Pd4 81.0(2) . .
Pd6 Pd2 Pd4 131.10(4) . .
Pd5 Pd2 Pd4 93.48(3) . .
Pd7 Pd2 Pd4 64.87(3) . .
O18 Pd2 K5 131.9(2) . .
O7 Pd2 K5 131.2(2) . .
O19 Pd2 K5 45.7(3) . .
O10 Pd2 K5 45.2(2) . .
Pd6 Pd2 K5 125.55(5) . .
Pd5 Pd2 K5 101.77(6) . .
Pd7 Pd2 K5 124.42(5) . .
Pd4 Pd2 K5 101.25(6) . .
O27 Pd3 O26 87.4(3) . .
O27 Pd3 O25 176.8(4) . .
O26 Pd3 O25 94.0(3) . .
O27 Pd3 O30 95.1(3) . .
O26 Pd3 O30 177.5(3) . .
O25 Pd3 O30 83.6(4) . .
O27 Pd3 Pd14 36.3(2) . .
O26 Pd3 Pd14 97.5(2) . .
O25 Pd3 Pd14 140.5(3) . .
O30 Pd3 Pd14 84.8(3) . .
O27 Pd3 K5 133.2(2) . .
O26 Pd3 K5 130.7(2) . .
O25 Pd3 K5 47.2(3) . .
O30 Pd3 K5 46.9(3) . .
Pd14 Pd3 K5 131.56(7) . .
O6 Pd4 O7 87.6(3) . .
O6 Pd4 O5 94.8(3) . .
O7 Pd4 O5 177.6(3) . .
O6 Pd4 O8 176.6(3) . .
O7 Pd4 O8 94.4(3) . .
O5 Pd4 O8 83.2(3) . .
O6 Pd4 Pd15 36.1(2) . .
O7 Pd4 Pd15 98.2(2) . .
O5 Pd4 Pd15 83.7(3) . .
O8 Pd4 Pd15 140.7(3) . .
O6 Pd4 Pd2 98.0(2) . .
O7 Pd4 Pd2 35.7(2) . .
O5 Pd4 Pd2 143.4(3) . .
O8 Pd4 Pd2 82.2(2) . .
Pd15 Pd4 Pd2 86.73(3) . .
O6 Pd4 K5 133.2(2) . 13_566
O7 Pd4 K5 129.7(2) . 13_566
O5 Pd4 K5 48.4(3) . 13_566
O8 Pd4 K5 46.7(2) . 13_566
Pd15 Pd4 K5 132.07(7) . 13_566
Pd2 Pd4 K5 128.89(6) . 13_566
O18 Pd5 O17 94.9(3) . .
O18 Pd5 O3 86.8(3) . .
O17 Pd5 O3 178.2(3) . .
O18 Pd5 O34 176.8(3) . .
O17 Pd5 O34 82.8(4) . .
O3 Pd5 O34 95.5(3) . .
O18 Pd5 Pd2 35.9(2) . .
O17 Pd5 Pd2 84.9(3) . .
O3 Pd5 Pd2 96.8(2) . .
O34 Pd5 Pd2 141.3(3) . .
O18 Pd5 K6 132.9(2) . .
O17 Pd5 K6 46.7(3) . .
O3 Pd5 K6 131.5(2) . .
O34 Pd5 K6 46.3(3) . .
Pd2 Pd5 K6 131.53(8) . .
O15 Pd6 O18 86.9(4) . .
O15 Pd6 O14 94.8(4) . .
O18 Pd6 O14 178.1(4) . .
O15 Pd6 O16 177.1(4) . .
O18 Pd6 O16 95.6(4) . .
O14 Pd6 O16 82.7(4) . .
O15 Pd6 Pd2 96.5(2) . .
O18 Pd6 Pd2 36.9(2) . .
O14 Pd6 Pd2 141.9(3) . .
O16 Pd6 Pd2 84.7(3) . .
O15 Pd6 Pd9 34.6(3) . .
O18 Pd6 Pd9 97.7(2) . .
O14 Pd6 Pd9 83.3(3) . .
O16 Pd6 Pd9 143.2(3) . .
Pd2 Pd6 Pd9 85.67(3) . .
O15 Pd6 K1 134.7(3) . .
O18 Pd6 K1 131.9(2) . .
O14 Pd6 K1 46.9(3) . .
O16 Pd6 K1 43.8(3) . .
Pd2 Pd6 K1 128.20(10) . .
Pd9 Pd6 K1 129.95(10) . .
O32 Pd7 O7 86.1(4) . .
O32 Pd7 O11 95.3(4) . .
O7 Pd7 O11 178.6(4) . .
O32 Pd7 O9 177.2(4) . .
O7 Pd7 O9 96.3(3) . .
O11 Pd7 O9 82.3(4) . .
O32 Pd7 Pd9 35.6(3) . .
O7 Pd7 Pd9 96.9(2) . .
O11 Pd7 Pd9 84.1(3) . .
O9 Pd7 Pd9 142.3(3) . .
O32 Pd7 Pd2 96.3(3) . .
O7 Pd7 Pd2 36.1(2) . .
O11 Pd7 Pd2 143.1(3) . .
O9 Pd7 Pd2 84.9(2) . .
Pd9 Pd7 Pd2 85.35(3) . .
O32 Pd7 K4 128.3(3) . 13_566
O7 Pd7 K4 126.9(2) . 13_566
O11 Pd7 K4 52.3(3) . 13_566
O9 Pd7 K4 51.0(3) . 13_566
Pd9 Pd7 K4 135.31(14) . 13_566
Pd2 Pd7 K4 134.46(14) . 13_566
O22 Pd8 O26 86.4(3) . .
O22 Pd8 O24 177.4(4) . .
O26 Pd8 O24 96.1(3) . .
O22 Pd8 O23 95.1(4) . .
O26 Pd8 O23 177.8(4) . .
O24 Pd8 O23 82.3(4) . .
O22 Pd8 Pd1 96.6(2) . .
O26 Pd8 Pd1 36.3(2) . .
O24 Pd8 Pd1 85.1(3) . .
O23 Pd8 Pd1 141.7(3) . .
O22 Pd8 Pd10 35.3(3) . .
O26 Pd8 Pd10 96.5(2) . .
O24 Pd8 Pd10 143.4(3) . .
O23 Pd8 Pd10 83.9(3) . .
Pd1 Pd8 Pd10 85.08(3) . .
O22 Pd8 K4 128.8(3) . .
O26 Pd8 K4 125.7(3) . .
O24 Pd8 K4 49.9(3) . .
O23 Pd8 K4 54.3(3) . .
Pd1 Pd8 K4 133.51(14) . .
Pd10 Pd8 K4 136.87(14) . .
O15 Pd9 O32 88.6(5) . .
O15 Pd9 O13 94.6(4) . .
O32 Pd9 O13 176.8(5) . .
O15 Pd9 O12 177.2(4) . .
O32 Pd9 O12 94.2(4) . .
O13 Pd9 O12 82.7(5) . .
O15 Pd9 Pd7 102.1(2) . 10_557
O32 Pd9 Pd7 35.78(12) . 10_557
O13 Pd9 Pd7 142.88(16) . 10_557
O12 Pd9 Pd7 80.2(3) . 10_557
O15 Pd9 Pd7 102.1(2) . .
O32 Pd9 Pd7 35.78(12) . .
O13 Pd9 Pd7 142.88(16) . .
O12 Pd9 Pd7 80.2(3) . .
Pd7 Pd9 Pd7 65.05(4) 10_557 .
O15 Pd9 Pd6 35.30(12) . .
O32 Pd9 Pd6 102.0(3) . .
O13 Pd9 Pd6 80.7(3) . .
O12 Pd9 Pd6 143.53(15) . .
Pd7 Pd9 Pd6 129.96(5) 10_557 .
Pd7 Pd9 Pd6 94.06(3) . .
O15 Pd9 Pd6 35.30(12) . 10_557
O32 Pd9 Pd6 102.0(3) . 10_557
O13 Pd9 Pd6 80.7(3) . 10_557
O12 Pd9 Pd6 143.53(15) . 10_557
Pd7 Pd9 Pd6 94.06(3) 10_557 10_557
Pd7 Pd9 Pd6 129.96(5) . 10_557
Pd6 Pd9 Pd6 64.21(4) . 10_557
O15 Pd9 K2 136.4(3) . 11_576
O32 Pd9 K2 135.0(3) . 11_576
O13 Pd9 K2 41.8(3) . 11_576
O12 Pd9 K2 40.9(3) . 11_576
Pd7 Pd9 K2 114.30(5) 10_557 11_576
Pd7 Pd9 K2 114.30(5) . 11_576
Pd6 Pd9 K2 115.74(5) . 11_576
Pd6 Pd9 K2 115.74(5) 10_557 11_576
O22 Pd10 O22 89.6(6) . 3
O22 Pd10 O21 176.8(5) . 3
O22 Pd10 O21 93.6(4) 3 3
O22 Pd10 O21 93.6(4) . .
O22 Pd10 O21 176.8(5) 3 .
O21 Pd10 O21 83.2(7) 3 .
O22 Pd10 Pd8 35.70(11) . .
O22 Pd10 Pd8 102.9(2) 3 .
O21 Pd10 Pd8 142.94(16) 3 .
O21 Pd10 Pd8 79.8(3) . .
O22 Pd10 Pd8 102.9(2) . 3
O22 Pd10 Pd8 35.70(11) 3 3
O21 Pd10 Pd8 79.8(3) 3 3
O21 Pd10 Pd8 142.94(16) . 3
Pd8 Pd10 Pd8 130.96(6) . 3
O22 Pd10 Pd8 35.70(11) . 10_556
O22 Pd10 Pd8 102.9(2) 3 10_556
O21 Pd10 Pd8 142.94(16) 3 10_556
O21 Pd10 Pd8 79.8(3) . 10_556
Pd8 Pd10 Pd8 64.90(3) . 10_556
Pd8 Pd10 Pd8 94.57(4) 3 10_556
O22 Pd10 Pd8 102.9(2) . 12
O22 Pd10 Pd8 35.70(11) 3 12
O21 Pd10 Pd8 79.8(3) 3 12
O21 Pd10 Pd8 142.94(16) . 12
Pd8 Pd10 Pd8 94.57(4) . 12
Pd8 Pd10 Pd8 64.90(3) 3 12
Pd8 Pd10 Pd8 130.96(6) 10_556 12
O22 Pd10 K3 135.2(3) . .
O22 Pd10 K3 135.2(3) 3 .
O21 Pd10 K3 41.6(3) 3 .
O21 Pd10 K3 41.6(3) . .
Pd8 Pd10 K3 114.52(3) . .
Pd8 Pd10 K3 114.52(3) 3 .
Pd8 Pd10 K3 114.52(3) 10_556 .
Pd8 Pd10 K3 114.52(3) 12 .
O27 Pd11 O27 86.3(4) 10_556 .
O27 Pd11 O28 178.4(4) 10_556 .
O27 Pd11 O28 95.1(3) . .
O27 Pd11 O28 95.1(3) 10_556 10_556
O27 Pd11 O28 178.4(4) . 10_556
O28 Pd11 O28 83.6(6) . 10_556
O27 Pd11 Pd14 35.9(2) 10_556 10_556
O27 Pd11 Pd14 97.9(2) . 10_556
O28 Pd11 Pd14 142.8(3) . 10_556
O28 Pd11 Pd14 82.7(3) 10_556 10_556
O27 Pd11 Pd14 97.9(2) 10_556 .
O27 Pd11 Pd14 35.9(2) . .
O28 Pd11 Pd14 82.7(3) . .
O28 Pd11 Pd14 142.8(3) 10_556 .
Pd14 Pd11 Pd14 87.75(4) 10_556 .
O27 Pd11 K2 134.0(2) 10_556 .
O27 Pd11 K2 134.0(2) . .
O28 Pd11 K2 45.2(3) . .
O28 Pd11 K2 45.2(3) 10_556 .
Pd14 Pd11 K2 127.49(5) 10_556 .
Pd14 Pd11 K2 127.49(5) . .
O6 Pd12 O6 85.9(4) . 10_557
O6 Pd12 O20 178.7(4) . 10_557
O6 Pd12 O20 95.1(3) 10_557 10_557
O6 Pd12 O20 95.1(3) . .
O6 Pd12 O20 178.7(4) 10_557 .
O20 Pd12 O20 83.9(5) 10_557 .
O6 Pd12 Pd15 35.7(2) . .
O6 Pd12 Pd15 97.1(2) 10_557 .
O20 Pd12 Pd15 143.2(3) 10_557 .
O20 Pd12 Pd15 83.3(2) . .
O6 Pd12 Pd15 97.1(2) . 10_557
O6 Pd12 Pd15 35.7(2) 10_557 10_557
O20 Pd12 Pd15 83.3(2) 10_557 10_557
O20 Pd12 Pd15 143.2(3) . 10_557
Pd15 Pd12 Pd15 86.56(4) . 10_557
O6 Pd12 K2 134.3(2) . 13_566
O6 Pd12 K2 134.3(2) 10_557 13_566
O20 Pd12 K2 45.1(2) 10_557 13_566
O20 Pd12 K2 45.1(2) . 13_566
Pd15 Pd12 K2 127.96(4) . 13_566
Pd15 Pd12 K2 127.96(4) 10_557 13_566
O3 Pd13 O3 86.3(4) 10_557 .
O3 Pd13 O55 178.6(3) 10_557 .
O3 Pd13 O55 94.8(3) . .
O3 Pd13 O55 94.8(3) 10_557 10_557
O3 Pd13 O55 178.6(3) . 10_557
O55 Pd13 O55 84.2(5) . 10_557
O3 Pd13 Pd15 35.7(2) 10_557 10_557
O3 Pd13 Pd15 97.1(2) . 10_557
O55 Pd13 Pd15 143.1(3) . 10_557
O55 Pd13 Pd15 83.3(2) 10_557 10_557
O3 Pd13 Pd15 97.1(2) 10_557 .
O3 Pd13 Pd15 35.7(2) . .
O55 Pd13 Pd15 83.3(2) . .
O55 Pd13 Pd15 143.1(3) 10_557 .
Pd15 Pd13 Pd15 86.40(4) 10_557 .
O3 Pd13 K3 130.4(2) 10_557 9_566
O3 Pd13 K3 130.4(2) . 9_566
O55 Pd13 K3 49.4(2) . 9_566
O55 Pd13 K3 49.4(2) 10_557 9_566
Pd15 Pd13 K3 132.43(4) 10_557 9_566
Pd15 Pd13 K3 132.43(4) . 9_566
O27 Pd14 O27 88.5(4) 12 .
O27 Pd14 O31 177.9(3) 12 .
O27 Pd14 O31 93.6(3) . .
O27 Pd14 O31 93.6(3) 12 12
O27 Pd14 O31 177.9(4) . 12
O31 Pd14 O31 84.3(5) . 12
O27 Pd14 Pd3 36.0(2) 12 12
O27 Pd14 Pd3 102.3(2) . 12
O31 Pd14 Pd3 143.2(3) . 12
O31 Pd14 Pd3 79.5(3) 12 12
O27 Pd14 Pd3 102.3(2) 12 .
O27 Pd14 Pd3 36.0(2) . .
O31 Pd14 Pd3 79.5(3) . .
O31 Pd14 Pd3 143.2(3) 12 .
Pd3 Pd14 Pd3 94.23(5) 12 .
O27 Pd14 Pd11 35.9(2) 12 3
O27 Pd14 Pd11 101.3(2) . 3
O31 Pd14 Pd11 143.2(3) . 3
O31 Pd14 Pd11 80.4(3) 12 3
Pd3 Pd14 Pd11 65.61(3) 12 3
Pd3 Pd14 Pd11 130.05(5) . 3
O27 Pd14 Pd11 101.3(2) 12 .
O27 Pd14 Pd11 35.9(2) . .
O31 Pd14 Pd11 80.4(3) . .
O31 Pd14 Pd11 143.2(3) 12 .
Pd3 Pd14 Pd11 130.05(5) 12 .
Pd3 Pd14 Pd11 65.61(3) . .
Pd11 Pd14 Pd11 92.25(4) 3 .
O6 Pd15 O3 87.6(3) . .
O6 Pd15 O33 177.8(3) . .
O3 Pd15 O33 94.6(3) . .
O6 Pd15 O4 93.5(3) . .
O3 Pd15 O4 178.9(3) . .
O33 Pd15 O4 84.3(4) . .
O6 Pd15 Pd4 36.0(2) . .
O3 Pd15 Pd4 100.7(2) . .
O33 Pd15 Pd4 143.4(3) . .
O4 Pd15 Pd4 80.1(3) . .
O6 Pd15 Pd12 35.8(2) . .
O3 Pd15 Pd12 101.4(2) . .
O33 Pd15 Pd12 143.1(3) . .
O4 Pd15 Pd12 79.6(3) . .
Pd4 Pd15 Pd12 65.42(3) . .
O6 Pd15 Pd13 101.2(2) . .
O3 Pd15 Pd13 35.7(2) . .
O33 Pd15 Pd13 80.5(3) . .
O4 Pd15 Pd13 144.1(3) . .
Pd4 Pd15 Pd13 129.08(4) . .
Pd12 Pd15 Pd13 93.46(3) . .
O12 Se1 O11 104.2(4) . 10_557
O12 Se1 O11 104.2(4) . .
O11 Se1 O11 103.0(7) 10_557 .
O12 Se1 K2 35.5(4) . 11_576
O11 Se1 K2 122.1(4) 10_557 11_576
O11 Se1 K2 122.1(4) . 11_576
O21 Se2 O23 104.2(4) . .
O21 Se2 O23 104.2(4) . 10_556
O23 Se2 O23 103.9(8) . 10_556
O13 Se3 O14 104.4(4) . .
O13 Se3 O14 104.4(4) . 10_557
O14 Se3 O14 103.2(8) . 10_557
O25 Se4 O29 105.6(4) . .
O25 Se4 O24 102.9(5) . .
O29 Se4 O24 102.7(4) . .
O25 Se4 K6 107.3(3) . .
O29 Se4 K6 37.1(3) . .
O24 Se4 K6 134.9(3) . .
O8 Se5 O10 104.8(4) . .
O8 Se5 O9 103.5(4) . .
O10 Se5 O9 103.8(4) . .
O8 Se5 K5 101.6(3) . .
O10 Se5 K5 38.0(3) . .
O9 Se5 K5 139.1(3) . .
O19 Se6 O17 105.5(4) . .
O19 Se6 O16 103.5(4) . .
O17 Se6 O16 101.6(5) . .
O28 Se7 O30 106.6(5) . .
O28 Se7 O31 103.6(5) . .
O30 Se7 O31 104.0(5) . .
O20 Se8 O4 103.7(4) . .
O20 Se8 O5 105.8(5) . .
O4 Se8 O5 103.9(5) . .
O55 Se9 O34 105.7(5) . .
O55 Se9 O33 104.9(4) . .
O34 Se9 O33 103.7(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
K1 O43 2.53(2) .
K1 O52 2.53(2) .
K1 O16 2.654(10) 12
K1 O16 2.654(10) .
K1 O14 2.762(9) .
K1 O14 2.762(9) 12
K1 O44 3.04(2) .
K1 O51 3.29(2) .
K1 Pd6 3.714(3) 12
K1 Pd6 3.714(3) .
K2 O12 2.730(12) 11_575
K2 O13 2.763(13) 11_575
K2 O28 2.790(10) 10_556
K2 O28 2.790(10) .
K2 O20 2.828(9) 13_566
K2 O20 2.828(9) 6_564
K2 O35 3.11(2) 10_556
K2 O35 3.11(2) .
K2 Pd11 3.819(4) .
K2 Pd12 3.862(4) 13_566
K2 Pd9 3.914(5) 11_575
K2 Se1 3.927(4) 11_575
K3 O21 2.775(14) .
K3 O21 2.775(14) 3
K3 O55 2.906(8) 2_564
K3 O55 2.906(8) 4_566
K3 O55 2.906(8) 9_566
K3 O55 2.906(8) 11_565
K3 O36 3.02(3) 10_556
K3 O36 3.02(3) .
K3 O37 3.23(3) .
K3 O37 3.23(3) 10_556
K3 Pd13 3.786(3) 11_565
K3 Pd13 3.786(3) 9_566
K4 O42 2.14(2) .
K4 O41 2.68(2) .
K4 O24 2.688(11) .
K4 O9 2.756(10) 13_566
K4 O49 2.80(2) .
K4 O11 2.802(11) 13_566
K4 O23 2.843(11) .
K4 Pd8 3.499(5) .
K4 Pd7 3.535(5) 13_566
K4 K4 4.616(18) 10_556
K4 K5 4.761(10) .
K5 O30 2.741(9) .
K5 O25 2.749(9) .
K5 O8 2.764(9) 13_566
K5 O10 2.796(9) .
K5 O19 2.811(9) .
K5 O41 2.817(18) .
K5 O5 2.824(9) 13_566
K5 O39 3.31(2) .
K5 O40 3.308(19) .
K5 Pd3 3.687(3) .
K5 Pd4 3.724(3) 13_566
K5 Pd2 3.821(3) .
K6 O29 2.763(10) 12
K6 O29 2.763(10) .
K6 O34 2.814(9) 12
K6 O34 2.814(9) .
K6 O17 2.831(9) .
K6 O17 2.831(9) 12
K6 O38 2.91(2) .
K6 O51 3.12(2) .
K6 O36 3.18(3) 9_566
K6 Pd5 3.799(2) .
K6 Pd5 3.799(2) 12
K6 Pd1 3.819(5) .
O3 Pd15 2.005(7) .
O3 Pd13 2.005(7) .
O3 Pd5 2.010(7) .
O4 Se8 1.687(9) .
O4 Pd15 2.033(9) .
O5 Se8 1.699(9) .
O5 Pd4 2.003(8) .
O5 K5 2.824(9) 13_566
O6 Pd4 1.997(7) .
O6 Pd15 2.003(7) .
O6 Pd12 2.004(7) .
O7 Pd4 1.997(8) .
O7 Pd7 2.006(8) .
O7 Pd2 2.008(7) .
O8 Se5 1.678(9) .
O8 Pd4 2.017(8) .
O8 K5 2.764(9) 13_566
O9 Se5 1.729(9) .
O9 Pd7 2.019(8) .
O9 K4 2.756(10) 13_566
O10 Se5 1.689(8) .
O10 Pd2 2.018(8) .
O11 Se1 1.703(10) .
O11 Pd7 2.012(9) .
O11 K4 2.802(11) 13_566
O12 Se1 1.697(11) .
O12 Pd9 2.013(12) .
O12 K2 2.730(12) 11_576
O13 Se3 1.707(12) .
O13 Pd9 2.010(12) .
O13 K2 2.763(13) 11_576
O14 Se3 1.709(10) .
O14 Pd6 2.005(9) .
O15 Pd9 1.967(10) .
O15 Pd6 2.001(5) .
O15 Pd6 2.001(5) 10_557
O16 Se6 1.724(10) .
O16 Pd6 2.016(9) .
O17 Se6 1.701(10) .
O17 Pd5 2.000(9) .
O18 Pd5 1.986(8) .
O18 Pd2 2.001(7) .
O18 Pd6 2.003(8) .
O19 Se6 1.674(8) .
O19 Pd2 2.015(8) .
O20 Se8 1.686(9) .
O20 Pd12 2.015(8) .
O20 K2 2.828(9) 13_566
O21 Se2 1.686(12) .
O21 Pd10 2.033(12) .
O22 Pd10 1.979(10) .
O22 Pd8 1.998(4) .
O22 Pd8 1.998(4) 10_556
O23 Se2 1.690(10) .
O23 Pd8 2.019(10) .
O24 Se4 1.735(10) .
O24 Pd8 2.016(9) .
O25 Se4 1.676(10) .
O25 Pd3 2.009(9) .
O26 Pd3 1.991(8) .
O26 Pd1 1.998(7) .
O26 Pd8 2.005(8) .
O27 Pd3 1.990(8) .
O27 Pd14 2.008(8) .
O27 Pd11 2.011(8) .
O28 Se7 1.681(10) .
O28 Pd11 2.027(9) .
O29 Se4 1.690(8) .
O29 Pd1 2.005(9) .
O30 Se7 1.697(10) .
O30 Pd3 2.009(9) .
O31 Se7 1.704(9) .
O31 Pd14 2.027(9) .
O32 Pd9 1.983(10) .
O32 Pd7 1.992(5) 10_557
O32 Pd7 1.992(5) .
O33 Se9 1.710(9) .
O33 Pd15 2.030(9) .
O34 Se9 1.695(10) .
O34 Pd5 2.015(9) .
O36 K6 3.18(3) 9_566
O42 O53 1.81(2) .
O49 K4 2.80(2) 10_556
O52 O52 1.27(4) 10_557
O55 Se9 1.679(9) .
O55 Pd13 2.024(8) .
O55 K3 2.906(8) 9_566
Pd1 O26 1.998(7) 12
Pd1 O29 2.005(9) 12
Pd1 Pd8 3.2231(11) 12
Pd1 Pd8 3.2231(11) .
Pd2 Pd6 3.1996(12) .
Pd2 Pd5 3.2359(12) .
Pd2 Pd7 3.2437(12) .
Pd2 Pd4 3.2565(12) .
Pd3 Pd14 3.2275(13) .
Pd4 Pd15 3.2353(13) .
Pd4 K5 3.724(3) 13_566
Pd6 Pd9 3.2528(13) .
Pd7 Pd9 3.2287(12) .
Pd7 K4 3.535(5) 13_566
Pd8 Pd10 3.2372(11) .
Pd9 Pd7 3.2287(12) 10_557
Pd9 Pd6 3.2528(13) 10_557
Pd9 K2 3.914(5) 11_576
Pd10 O22 1.979(10) 3
Pd10 O21 2.033(12) 3
Pd10 Pd8 3.2372(11) 3
Pd10 Pd8 3.2372(11) 10_556
Pd10 Pd8 3.2372(11) 12
Pd11 O27 2.011(8) 10_556
Pd11 O28 2.027(9) 10_556
Pd11 Pd14 3.2555(13) 10_556
Pd11 Pd14 3.2555(13) .
Pd12 O6 2.004(7) 10_557
Pd12 O20 2.015(8) 10_557
Pd12 Pd15 3.2515(12) .
Pd12 Pd15 3.2515(12) 10_557
Pd12 K2 3.862(4) 13_566
Pd13 O3 2.005(7) 10_557
Pd13 O55 2.024(8) 10_557
Pd13 Pd15 3.2564(12) 10_557
Pd13 Pd15 3.2564(12) .
Pd13 K3 3.786(3) 9_566
Pd14 O27 2.008(8) 12
Pd14 O31 2.027(9) 12
Pd14 Pd3 3.2275(13) 12
Pd14 Pd11 3.2555(13) 3
Se1 O11 1.703(10) 10_557
Se1 K2 3.927(4) 11_576
Se2 O23 1.690(10) 10_556
Se3 O14 1.709(10) 10_557
